Download presentation

Presentation is loading. Please wait.

Published byKelly Weaver Modified about 1 year ago

1
Estimating Crystallite Size Using XRD Scott A Speakman, Ph.D A MIT Center for Materials Science and Engineering

2
Center for Materials Science and Engineering Warning These slides have not been extensively proof-read, and therefore may contain errors. While I have tried to cite all references, I may have missed some– these slides were prepared for an informal lecture and not for publication. If you note a mistake or a missing citation, please let me know and I will correct it. I hope to add commentary in the notes section of these slides, offering additional details. However, these notes are incomplete so far.

3
Center for Materials Science and Engineering Goals of Today’s Lecture Provide a quick overview of the theory behind peak profile analysis Discuss practical considerations for analysis Demonstrate the use of lab software for analysis –empirical peak fitting using MDI Jade –Rietveld refinement using HighScore Plus Discuss other software for peak profile analysis Briefly mention other peak profile analysis methods –Warren Averbach Variance method –Mixed peak profiling –whole pattern Discuss other ways to evaluate crystallite size Assumptions: you understand the basics of crystallography, X-ray diffraction, and the operation of a Bragg-Brentano diffractometer

4
Center for Materials Science and Engineering A Brief History of XRD Röntgen publishes the discovery of X-rays Laue observes diffraction of X-rays from a crystal when did Scherrer use X-rays to estimate the crystallite size of nanophase materials?when did Scherrer use X-rays to estimate the crystallite size of nanophase materials?

5
Center for Materials Science and Engineering The Scherrer Equation was published in 1918 Peak width (B) is inversely proportional to crystallite size (L) P. Scherrer, “Bestimmung der Grösse und der inneren Struktur von Kolloidteilchen mittels Röntgenstrahlen,” Nachr. Ges. Wiss. Göttingen 26 (1918) pp J.I. Langford and A.J.C. Wilson, “Scherrer after Sixty Years: A Survey and Some New Results in the Determination of Crystallite Size,” J. Appl. Cryst. 11 (1978) pp

6
Center for Materials Science and Engineering The Laue Equations describe the intensity of a diffracted peak from a single parallelopipeden crystal N 1, N 2, and N 3 are the number of unit cells along the a 1, a 2, and a 3 directions When N is small, the diffraction peaks become broader The peak area remains constant independent of N

7
Center for Materials Science and Engineering Which of these diffraction patterns comes from a nanocrystalline material? (deg.) Intensity (a.u.) These diffraction patterns were produced from the exact same sample Two different diffractometers, with different optical configurations, were used The apparent peak broadening is due solely to the instrumentation

8
Center for Materials Science and Engineering Many factors may contribute to the observed peak profile Instrumental Peak Profile Crystallite Size Microstrain –Non-uniform Lattice Distortions –Faulting –Dislocations –Antiphase Domain Boundaries –Grain Surface Relaxation Solid Solution Inhomogeneity Temperature Factors The peak profile is a convolution of the profiles from all of these contributionsThe peak profile is a convolution of the profiles from all of these contributions

9
Center for Materials Science and Engineering Instrument and Sample Contributions to the Peak Profile must be Deconvoluted In order to analyze crystallite size, we must deconvolute: –Instrumental Broadening FW(I) also referred to as the Instrumental Profile, Instrumental FWHM Curve, Instrumental Peak Profile –Specimen Broadening FW(S) also referred to as the Sample Profile, Specimen Profile We must then separate the different contributions to specimen broadening –Crystallite size and microstrain broadening of diffraction peaks

10
Center for Materials Science and Engineering Contributions to Peak Profile 1.Peak broadening due to crystallite size 2.Peak broadening due to the instrumental profile 3.Which instrument to use for nanophase analysis 4.Peak broadening due to microstrain the different types of microstrain Peak broadening due to solid solution inhomogeneity and due to temperature factors

11
Center for Materials Science and Engineering Crystallite Size Broadening Peak Width due to crystallite size varies inversely with crystallite size –as the crystallite size gets smaller, the peak gets broader The peak width varies with 2 as cos –The crystallite size broadening is most pronounced at large angles 2Theta However, the instrumental profile width and microstrain broadening are also largest at large angles 2theta peak intensity is usually weakest at larger angles 2theta –If using a single peak, often get better results from using diffraction peaks between 30 and 50 deg 2theta below 30deg 2theta, peak asymmetry compromises profile analysis

12
Center for Materials Science and Engineering The Scherrer Constant, K The constant of proportionality, K (the Scherrer constant) depends on the how the width is determined, the shape of the crystal, and the size distribution –the most common values for K are: 0.94 for FWHM of spherical crystals with cubic symmetry 0.89 for integral breadth of spherical crystals w/ cubic symmetry 1, because 0.94 and 0.89 both round up to 1 –K actually varies from 0.62 to 2.08 For an excellent discussion of K, refer to JI Langford and AJC Wilson, “Scherrer after sixty years: A survey and some new results in the determination of crystallite size,” J. Appl. Cryst. 11 (1978) p

13
Center for Materials Science and Engineering Factors that affect K and crystallite size analysis how the peak width is defined how crystallite size is defined the shape of the crystal the size distribution

14
Center for Materials Science and Engineering (deg.) Intensity (a.u.) Methods used in Jade to Define Peak Width Full Width at Half Maximum (FWHM) –the width of the diffraction peak, in radians, at a height half-way between background and the peak maximum Integral Breadth –the total area under the peak divided by the peak height –the width of a rectangle having the same area and the same height as the peak –requires very careful evaluation of the tails of the peak and the background (deg.) Intensity (a.u.) FWHM

15
Center for Materials Science and Engineering Integral Breadth Warren suggests that the Stokes and Wilson method of using integral breadths gives an evaluation that is independent of the distribution in size and shape –L is a volume average of the crystal thickness in the direction normal to the reflecting planes –The Scherrer constant K can be assumed to be 1 Langford and Wilson suggest that even when using the integral breadth, there is a Scherrer constant K that varies with the shape of the crystallites

16
Center for Materials Science and Engineering Other methods used to determine peak width These methods are used in more the variance methods, such as Warren-Averbach analysis –Most often used for dislocation and defect density analysis of metals –Can also be used to determine the crystallite size distribution –Requires no overlap between neighboring diffraction peaks Variance-slope –the slope of the variance of the line profile as a function of the range of integration Variance-intercept –negative initial slope of the Fourier transform of the normalized line profile

17
Center for Materials Science and Engineering How is Crystallite Size Defined Usually taken as the cube root of the volume of a crystallite –assumes that all crystallites have the same size and shape For a distribution of sizes, the mean size can be defined as –the mean value of the cube roots of the individual crystallite volumes –the cube root of the mean value of the volumes of the individual crystallites Scherrer method (using FWHM) gives the ratio of the root-mean- fourth-power to the root-mean-square value of the thickness Stokes and Wilson method (using integral breadth) determines the volume average of the thickness of the crystallites measured perpendicular to the reflecting plane The variance methods give the ratio of the total volume of the crystallites to the total area of their projection on a plane parallel to the reflecting planes

18
Center for Materials Science and Engineering Remember, Crystallite Size is Different than Particle Size A particle may be made up of several different crystallites Crystallite size often matches grain size, but there are exceptions

19
Center for Materials Science and Engineering Crystallite Shape Though the shape of crystallites is usually irregular, we can often approximate them as: –sphere, cube, tetrahedra, or octahedra –parallelepipeds such as needles or plates –prisms or cylinders Most applications of Scherrer analysis assume spherical crystallite shapes If we know the average crystallite shape from another analysis, we can select the proper value for the Scherrer constant K Anistropic peak shapes can be identified by anistropic peak broadening –if the dimensions of a crystallite are 2x * 2y * 200z, then (h00) and (0k0) peaks will be more broadened then (00l) peaks.

20
Center for Materials Science and Engineering Anistropic Size Broadening The broadening of a single diffraction peak is the product of the crystallite dimensions in the direction perpendicular to the planes that produced the diffraction peak.

21
Center for Materials Science and Engineering Crystallite Size Distribution is the crystallite size narrowly or broadly distributed? is the crystallite size unimodal? XRD is poorly designed to facilitate the analysis of crystallites with a broad or multimodal size distribution Variance methods, such as Warren-Averbach, can be used to quantify a unimodal size distribution –Otherwise, we try to accommodate the size distribution in the Scherrer constant –Using integral breadth instead of FWHM may reduce the effect of crystallite size distribution on the Scherrer constant K and therefore the crystallite size analysis

22
Center for Materials Science and Engineering Instrumental Peak Profile A large crystallite size, defect-free powder specimen will still produce diffraction peaks with a finite width The peak widths from the instrument peak profile are a convolution of: –X-ray Source Profile Wavelength widths of K 1 and K 2 lines Size of the X-ray source Superposition of K 1 and K 2 peaks –Goniometer Optics Divergence and Receiving Slit widths Imperfect focusing Beam size Penetration into the sample (deg.) Intensity (a.u.) Patterns collected from the same sample with different instruments and configurations at MIT

23
Center for Materials Science and Engineering What Instrument to Use? The instrumental profile determines the upper limit of crystallite size that can be evaluated –if the Instrumental peak width is much larger than the broadening due to crystallite size, then we cannot accurately determine crystallite size –For analyzing larger nanocrystallites, it is important to use the instrument with the smallest instrumental peak width Very small nanocrystallites produce weak signals –the specimen broadening will be significantly larger than the instrumental broadening –the signal:noise ratio is more important than the instrumental profile

24
Center for Materials Science and Engineering Comparison of Peak Widths at 47 ° 2 for Instruments and Crystallite Sizes Rigaku XRPD is better for very small nanocrystallites, <80 nm (upper limit 100 nm) PANalytical X’Pert Pro is better for larger nanocrystallites, <150 nm ConfigurationFWHM (deg) Pk Ht to Bkg Ratio Rigaku, LHS, 0.5° DS, 0.3mm RS Rigaku, LHS, 1° DS, 0.3mm RS Rigaku, RHS, 0.5° DS, 0.3mm RS Rigaku, RHS, 1° DS, 0.3mm RS X’Pert Pro, High-speed, 0.25° DS X’Pert Pro, High-speed, 0.5° DS X’Pert, 0.09° Parallel Beam Collimator X’Pert, 0.27° Parallel Beam Collimator Crystallite Size FWHM (deg) 100 nm nm nm nm1.745

25
Center for Materials Science and Engineering Other Instrumental Considerations for Thin Films The irradiated area greatly affects the intensity of high angle diffraction peaks –GIXD or variable divergence slits on the PANalytical X’Pert Pro will maintain a constant irradiated area, increasing the signal for high angle diffraction peaks –both methods increase the instrumental FWHM Bragg-Brentano geometry only probes crystallite dimensions through the thickness of the film –in order to probe lateral (in-plane) crystallite sizes, need to collect diffraction patterns at different tilts –this requires the use of parallel-beam optics on the PANalytical X’Pert Pro, which have very large FWHM and poor signal:noise ratios

26
Center for Materials Science and Engineering Microstrain Broadening lattice strains from displacements of the unit cells about their normal positions often produced by dislocations, domain boundaries, surfaces etc. microstrains are very common in nanocrystalline materials the peak broadening due to microstrain will vary as: compare to peak broadening due to crystallite size:

27
Center for Materials Science and Engineering Contributions to Microstrain Broadening Non-uniform Lattice Distortions Dislocations Antiphase Domain Boundaries Grain Surface Relaxation Other contributions to broadening –faulting –solid solution inhomogeneity –temperature factors

28
Center for Materials Science and Engineering Non-Uniform Lattice Distortions Rather than a single d-spacing, the crystallographic plane has a distribution of d-spaces This produces a broader observed diffraction peak Such distortions can be introduced by: –surface tension of nanocrystals –morphology of crystal shape, such as nanotubes –interstitial impurities (deg.) Intensity (a.u.)

29
Center for Materials Science and Engineering Antiphase Domain Boundaries Formed during the ordering of a material that goes through an order-disorder transformation The fundamental peaks are not affected the superstructure peaks are broadened –the broadening of superstructure peaks varies with hkl

30
Center for Materials Science and Engineering Dislocations Line broadening due to dislocations has a strong hkl dependence The profile is Lorentzian Can try to analyze by separating the Lorentzian and Gaussian components of the peak profile Can also determine using the Warren-Averbach method –measure several orders of a peak 001, 002, 003, 004, … 110, 220, 330, 440, … –The Fourier coefficient of the sample broadening will contain an order independent term due to size broadening an order dependent term due to strain

31
Center for Materials Science and Engineering Faulting Broadening due to deformation faulting and twin faulting will convolute with the particle size Fourier coefficient –The particle size coefficient determined by Warren-Averbach analysis actually contains contributions from the crystallite size and faulting –the fault contribution is hkl dependent, while the size contribution should be hkl independent (assuming isotropic crystallite shape) –the faulting contribution varies as a function of hkl dependent on the crystal structure of the material (fcc vs bcc vs hcp) –See Warren, 1969, for methods to separate the contributions from deformation and twin faulting

32
Center for Materials Science and Engineering CeO 2 19 nm (deg.) Intensity (a.u.) ZrO 2 46nm Ce x Zr 1-x O 2 0

33
Center for Materials Science and Engineering Temperature Factor The Debye-Waller temperature factor describes the oscillation of an atom around its average position in the crystal structure The thermal agitation results in intensity from the peak maxima being redistributed into the peak tails –it does not broaden the FWHM of the diffraction peak, but it does broaden the integral breadth of the diffraction peak The temperature factor increases with 2Theta The temperature factor must be convoluted with the structure factor for each peak –different atoms in the crystal may have different temperature factors –each peak contains a different contribution from the atoms in the crystal

34
Center for Materials Science and Engineering Determining the Sample Broadening due to crystallite size The sample profile FW(S) can be deconvoluted from the instrumental profile FW(I) either numerically or by Fourier transform In Jade size and strain analysis –you individually profile fit every diffraction peak –deconvolute FW(I) from the peak profile functions to isolate FW(S) –execute analyses on the peak profile functions rather than on the raw data Jade can also use iterative folding to deconvolute FW(I) from the entire observed diffraction pattern –this produces an entire diffraction pattern without an instrumental contribution to peak widths –this does not require fitting of individual diffraction peaks –folding increases the noise in the observed diffraction pattern Warren Averbach analyses operate on the Fourier transform of the diffraction peak –take Fourier transform of peak profile functions or of raw data

35
Center for Materials Science and Engineering Analysis using MDI Jade The data analysis package Jade is designed to use empirical peak profile fitting to estimate crystallite size and/or microstrain Three Primary Components –Profile Fitting Techniques –Instrumental FWHM Curve –Size & Strain Analysis Scherrer method Williamson-Hall method

36
Center for Materials Science and Engineering Important Chapters in Jade Help Jade’s User Interface –User Preferences Dialog Advanced Pattern Processing –Profile Fitting and Peak Decomposition –Crystallite Size & Strain Analysis

37
Center for Materials Science and Engineering Profile Fitting Empirically fit experimental data with a series of equations –fit the diffraction peak using the profile function –fit background, usually as a linear segment this helps to separate intensity in peak tails from background To extract information, operate explicitly on the equation rather than numerically on the raw data Profile fitting produces precise peak positions, widths, heights, and areas with statistically valid estimates

38
Center for Materials Science and Engineering Profile Functions Diffraction peaks are usually the convolution of Gaussian and Lorentzian components Some techniques try to deconvolute the Gaussian and Lorentzian contributions to each diffraction peak; this is very difficult More typically, data are fit with a profile function that is a pseudo-Voigt or Pearson VII curve –pseudo-Voigt is a linear combination of Gaussian and Lorentzian components a true Voigt curve is a convolution of the Gaussian and Lorentzian components; this is more difficult to implement computationally –Pearson VII is an exponential mixing of Gaussian and Lorentzian components SA Howard and KD Preston, “Profile Fitting of Powder Diffraction Patterns,”, Reviews in Mineralogy vol 20: Modern Powder Diffraction, Mineralogical Society of America, Washington DC, 1989.

39
Center for Materials Science and Engineering Important Tips for Profile Fitting Do not process the data before profile fitting –do not smooth the data –do not fit and remove the background –do not strip Ka 2 peaks Load the appropriate PDF reference patterns for your phases of interest Zoom in so that as few peaks as possible, plus some background, is visible –Fit as few peaks simultaneously as possible –preferably fit only 1 peak at a time Constrain variables when necessary to enhance the stability of the refinement

40
Center for Materials Science and Engineering To Access the Profile Fitting Dialogue Window Menu: Analyze > Fit Peak Profile Right-click Fit Profiles button Right-click Profile Edit Cursor button

41
Center for Materials Science and Engineering open Ge103.xrdml overlay PDF reference pattern Demonstrate profile fitting of the 5 diffraction peaks –fit one at a time –fit using ‘All’ option

42
Center for Materials Science and Engineering Important Options in Profile Fitting Window

43
Center for Materials Science and Engineering 1. Profile Shape Function select the equation that will be used to fit diffraction peaks Gaussian: –more appropriate for fitting peaks with a rounder top –strain distribution tends to broaden the peak as a Gaussian Lorentzian: –more appropriate for fitting peaks with a sharper top –size distribution tends to broaden the peak as a Lorentzian –dislocations also create a Lorentzian component to the peak broadening The instrumental profile and peak shape are often a combination of Gaussian and Lorentzian contributions pseudo-Voigt: –emphasizes Guassian contribution –preferred when strain broadening dominates Pearson VII: –emphasize Lorentzian contribution –preferred when size broadening dominates

44
Center for Materials Science and Engineering 2. Shape Parameter This option allows you to constrain or refine the shape parameter –the shape parameter determines the relative contributions of Gaussian and Lorentzian type behavior to the profile function shape parameter is different for pseudo-Voigt and Pearson VII functions –pseudo-Voigt: sets the Lorentzian coefficient –Pearson VII: set the exponent Check the box if you want to constrain the shape parameter to a value –input the value that you want for the shape parameter in the numerical field Do not check the box if you want the mixing parameter to be refined during profile fitting –this is the much more common setting for this option

45
Center for Materials Science and Engineering 3. Skewness Skewness is used to model asymmetry in the diffraction peak –Most significant at low values of 2 Unchecked: skewness will be refined during profile fitting Checked: skewness will be constrained to the value indicated –usually check this option to constrain skewness to 0 –skewness=0 indicates a symmetrical peak Hint: constrain skewness to zero when –refining very broad peaks –refining very weak peaks –refining several heavily overlapping peaks an example of the error created when fitting low angle asymmetric data with a skewness=0 profile (deg.) Intensity (a.u.)

46
Center for Materials Science and Engineering (deg.) Intensity (a.u.) > Silicon - Si 4. K-alpha2 contribution Checking this box indicates that K 2 radiation is present and should be included in the peak profile model –this should almost always be checked when analyzing your data It is much more accurate to model K 2 than it is to numerically strip the K 2 contribution from the experimental data This is a single diffraction peak, featuring the K 1 and K 2 doublet

47
Center for Materials Science and Engineering (deg.) Intensity (a.u.) 5. Background function Specifies how the background underneath the peak will be modeled –usually use “Linear Background” –“Level Background” is appropriate if the background is indeed fairly level and the broadness of the peak causes the linear background function to fit improperly –manually fit the background (Analyze > Fit Background) and use “Fixed Background” for very complicated patterns –more complex background functions will usually fail when fitting nanocrystalline materials This linear background fit modeled the background too low. A level fit would not work, so the fixed background must be used.

48
Center for Materials Science and Engineering (deg.) Intensity (a.u.) 6. Initial Peak Width 7. Initial Peak Location These setting determine the way that Jade calculates the initial peak profile, before refinement Initial Width –if the peak is not significantly broadened by size or strain, then use the FWHM curve –if the peak is significantly broadened, you might have more success if you Specify a starting FWHM Initial Location –using PDF overlays is always the preferred option –if no PDF reference card is available, and the peak is significantly broadened, then you will want to manually insert peaks- the Peak Search will not work Result of auto insertion using peak search and FWHM curve on a nanocrystalline broadened peak. Manual peak insertion should be used instead.

49
Center for Materials Science and Engineering 8. Display Options Check the options for what visual components you want displayed during the profile fitting –Typically use: Overall Profile Individual Profiles Background Curve Line Marker –Sometimes use: Difference Pattern Paint Individuals

50
Center for Materials Science and Engineering 9. Fitting Results This area displays the results for profile fit peaks Numbers in () are estimated standard deviations (ESD) –if the ESD is marked with (?), then that peak profile function has not yet been refined Click once on a row, and the Main Display Area of Jade will move to show you that peak, and a blinking cursor will highlight that peak You can sort the peak fits by any column by clicking on the column header

51
Center for Materials Science and Engineering Other buttons of interest Execute Refinement Autofit All Peaks See Other Options Help Save Text File of Results

52
Center for Materials Science and Engineering Clicking Other Options Unify Variables: force all peaks to be fit using the same profile parameter Use FWHM or Integral Breadth for Crystallite Size Analysis Select What Columns to Show in the Results Area

53
Center for Materials Science and Engineering Procedure for Profile Fitting a Diffraction Pattern 1.Open the diffraction pattern 2.Overlay the PDF reference 3.Zoom in on first peak(s) to analyze 4.Open the profile fitting dialogue to configure options 5.Refine the profile fit for the first peak(s) 6.Review the quality of profile fit 7.Move to next peak(s) and profile fit 8.Continue until entire pattern is fit

54
Center for Materials Science and Engineering Procedure for Profile Fitting 1. Open the XRD pattern 2. Overlay PDF reference for the sample (deg.) Intensity (a.u.) > Aragonite - CaCO 3

55
Center for Materials Science and Engineering Procedure for Profile Fitting 3. Zoom in on First Peak to Analyze –try to zoom in on only one peak –be sure to include some background on either side of the peak (deg.) Intensity (a.u.) > Aragonite - CaCO 3

56
Center for Materials Science and Engineering Procedure for Profile Fitting when you open the profile fitting dialogue, an initial peak profile curve will be generated if the initial profile is not good, because initial width and location parameters were not yet set, then delete it –highlight the peak in the fitting results –press the delete key on your keyboard 4. Open profile fitting dialogue to configure parameter 5. Once parameters are configured properly, click on the blue triangle to execute “Profile Fitting” you may have to execute the refinement multiple times if the initial refinement stops before the peak is sufficiently fit

57
Center for Materials Science and Engineering Procedure for Profile Fitting 6. Review Quality of Profile Fit The least-squares fitting residual, R, will be listed in upper right corner of screen –the residual R should be less than 10% The ESD for parameters such as 2-Theta and FWHM should be small, in the last significant figure

58
Center for Materials Science and Engineering (deg.) Intensity (a.u.) > Aragonite - CaCO 3 Procedure for Profile Fitting 7. Move to Next Peak(s) In this example, peaks are too close together to refine individually Therefore, profile fit the group of peaks together Profile fitting, if done well, can help to separate overlapping peaks

59
Center for Materials Science and Engineering Procedure for Profile Fitting 8. Continue until the entire pattern is fit The results window will list a residual R for the fitting of the entire diffraction pattern The difference plot will highlight any major discrepancies

60
Center for Materials Science and Engineering Instrumental FWHM Calibration Curve The instrument itself contributes to the peak profile Before profile fitting the nanocrystalline phase(s) of interest –profile fit a calibration standard to determine the instrumental profile Important factors for producing a calibration curve –Use the exact same instrumental conditions same optical configuration of diffractometer same sample preparation geometry calibration curve should cover the 2theta range of interest for the specimen diffraction pattern –do not extrapolate the calibration curve

61
Center for Materials Science and Engineering Instrumental FWHM Calibration Curve Standard should share characteristics with the nanocrystalline specimen –similar mass absorption coefficient –similar atomic weight –similar packing density The standard should not contribute to the diffraction peak profile –macrocrystalline: crystallite size larger than 500 nm –particle size less than 10 microns –defect and strain free There are several calibration techniques –Internal Standard –External Standard of same composition –External Standard of different composition

62
Center for Materials Science and Engineering Internal Standard Method for Calibration Mix a standard in with your nanocrystalline specimen a NIST certified standard is preferred –use a standard with similar mass absorption coefficient –NIST 640c Si –NIST 660a LaB 6 –NIST 674b CeO 2 –NIST 675 Mica standard should have few, and preferably no, overlapping peaks with the specimen –overlapping peaks will greatly compromise accuracy of analysis

63
Center for Materials Science and Engineering Internal Standard Method for Calibration Advantages: –know that standard and specimen patterns were collected under identical circumstances for both instrumental conditions and sample preparation conditions –the linear absorption coefficient of the mixture is the same for standard and specimen Disadvantages: –difficult to avoid overlapping peaks between standard and broadened peaks from very nanocrystalline materials –the specimen is contaminated –only works with a powder specimen

64
Center for Materials Science and Engineering External Standard Method for Calibration If internal calibration is not an option, then use external calibration Run calibration standard separately from specimen, keeping as many parameters identical as is possible The best external standard is a macrocrystalline specimen of the same phase as your nanocrystalline specimen –How can you be sure that macrocrystalline specimen does not contribute to peak broadening?

65
Center for Materials Science and Engineering Qualifying your Macrocrystalline Standard select powder for your potential macrocrystalline standard –if not already done, possibly anneal it to allow crystallites to grow and to allow defects to heal use internal calibration to validate that macrocrystalline specimen is an appropriate standard –mix macrocrystalline standard with appropriate NIST SRM –compare FWHM curves for macrocrystalline specimen and NIST standard –if the macrocrystalline FWHM curve is similar to that from the NIST standard, than the macrocrystalline specimen is suitable –collect the XRD pattern from pure sample of you macrocrystalline specimen do not use the FHWM curve from the mixture with the NIST SRM

66
Center for Materials Science and Engineering Disadvantages/Advantages of External Calibration with a Standard of the Same Composition Advantages: –will produce better calibration curve because mass absorption coefficient, density, molecular weight are the same as your specimen of interest –can duplicate a mixture in your nanocrystalline specimen –might be able to make a macrocrystalline standard for thin film samples Disadvantages: –time consuming –desire a different calibration standard for every different nanocrystalline phase and mixture –macrocrystalline standard may be hard/impossible to produce –calibration curve will not compensate for discrepancies in instrumental conditions or sample preparation conditions between the standard and the specimen

67
Center for Materials Science and Engineering External Standard Method of Calibration using a NIST standard As a last resort, use an external standard of a composition that is different than your nanocrystalline specimen –This is actually the most common method used –Also the least accurate method Use a certified NIST standard to produce instrumental FWHM calibration curve

68
Center for Materials Science and Engineering Advantages and Disadvantages of using NIST standard for External Calibration Advantages –only need to build one calibration curve for each instrumental configuration –I have NIST standard diffraction patterns for each instrument and configuration available for download from –know that the standard is high quality if from NIST –neither standard nor specimen are contaminated Disadvantages –The standard may behave significantly different in diffractometer than your specimen different mass absorption coefficient different depth of penetration of X-rays –NIST standards are expensive –cannot duplicate exact conditions for thin films

69
Center for Materials Science and Engineering Consider- when is good calibration most essential? For a very small crystallite size, the specimen broadening dominates over instrumental broadening Only need the most exacting calibration when the specimen broadening is small because the specimen is not highly nanocrystalline FWHM of Instrumental Profile at 48° 2 deg Broadening Due to Nanocrystalline Size Crystallite Size B(2 ) (rad) FWHM (deg) 100 nm nm nm nm

70
Center for Materials Science and Engineering Steps for Producing an Instrumental Profile 1.Collect data from calibration standard 2.Profile fit peaks from the calibration standard 3.Produce FWHM curve 4.Save FWHM curve 5.Set software preferences to use FHWH curve as Instrumental Profile

71
Center for Materials Science and Engineering Steps for Producing an Instrumental Profile 1.Collect XRD pattern from standard over a long range 2.Profile fit all peaks of the standard’s XRD pattern use the profile function (Pearson VII or pseudo-Voigt) that you will use to fit your specimen pattern indicate if you want to use FWHM or Integral Breadth when analyzing specimen pattern 3.Produce a FWHM curve go to Analyze > FWHM Curve Plot

72
Center for Materials Science and Engineering Steps for Producing an Instrumental Profile 4. Save the FWHM curve go to File > Save > FWHM Curve of Peaks give the FWHM curve a name that you will be able to find again –the FWHM curve is saved in a database on the local computer –you need to produce the FWHM curve on each computer that you use –everybody else’s FHWM curves will also be visible

73
Center for Materials Science and Engineering Steps for Producing an Instrumental Profile 5. Set preferences to use the FWHM curve as the instrumental profile Go to Edit > Preferences Select the Instrument tab Select your FWHM curve from the drop-down menu on the bottom of the dialogue Also enter Goniometer Radius –Rigaku Right-Hand Side: 185mm –Rigaku Left-Hand Side: 250mm –PANalytical X’Pert Pro: 240mm

74
Center for Materials Science and Engineering Other Software Preferences That You Should Be Aware Of Report Tab –Check to calculate Crystallite Size from FWHM –set Scherrer constant Display tab –Check the last option to have crystallite sizes reported in nanometers –Do not check last option to have crystallite sizes reported in Angstroms

75
Center for Materials Science and Engineering Using the Scherrer Method in Jade to Estimate Crystallite Size load specimen data load PDF reference pattern Profile fit as many peaks of your data that you can (deg.) Intensity (a.u.) > Cerianite- - CeO 2

76
Center for Materials Science and Engineering Scherrer Analysis Calculates Crystallite Size based on each Individual Peak Profile Crystallite Size varies from 22 to 30 Å over the range of 28.5 to 95.4° 2 –Average size: 25 Å –Standard Deviation: 3.4 Å Pretty good analysis Not much indicator of crystallite strain We might use a single peak in future analyses, rather than all 8

77
Center for Materials Science and Engineering FWHM vs Integral Breadth Using FWHM: 25.1 Å (3.4) Using Breadth: 22.5 Å (3.7) Breadth not as accurate because there is a lot of overlap between peaks- cannot determine where tail intensity ends and background begins

78
Center for Materials Science and Engineering Analysis Using Different Values of K For the typical values of 0.81 < K < 1.03 –the crystallite size varies between 22 and 29 Å –The precision of XRD analysis is never better than ±1 nm –The size is reproducibly calculated as 2-3 nm K Avg

79
Center for Materials Science and Engineering For Size & Strain Analysis using Williamson- Hull type Plot in Jade after profile fitting all peaks, click size-strain button –or in main menus, go to Analyze > Size&Strain Plot

80
Center for Materials Science and Engineering Williamson Hull Plot y-intercept slope FW(S)*Cos(Theta) Sin(Theta) *Fit Size/Strain: XS(Å) = 33 (1), Strain(%) = (0.0343), ESD of Fit = , LC = 0.751

81
Center for Materials Science and Engineering Manipulating Options in the Size-Strain Plot of Jade 1.Select Mode of Analysis Fit Size/Strain Fit Size Fit Strain 2.Select Instrument Profile Curve 3.Show Origin 4.Deconvolution Parameter 5.Results 6.Residuals for Evaluation of Fit 7.Export or Save

82
Center for Materials Science and Engineering Analysis Mode: Fit Size Only slope= 0= strain FW(S)*Cos(Theta) Sin(Theta) *Fit Size Only: XS(Å) = 26 (1), Strain(%) = 0.0, ESD of Fit = , LC = 0.751

83
Center for Materials Science and Engineering Analysis Mode: Fit Strain Only y-intercept= 0 size= ∞ FW(S)*Cos(Theta) Sin(Theta) *Fit Strain Only: XS(Å) = 0, Strain(%) = (0.0112), ESD of Fit = , LC = 0.751

84
Center for Materials Science and Engineering Analysis Mode: Fit Size/Strain FW(S)*Cos(Theta) Sin(Theta) *Fit Size/Strain: XS(Å) = 33 (1), Strain(%) = (0.0343), ESD of Fit = , LC = 0.751

85
Center for Materials Science and Engineering Comparing Results Size (A)Strain (%)ESD of Fit Size(A)Strain(%)ESD of Fit Size Only 22(1) (1) Strain Only -4.03(1) (1) Size & Strain 28(1)0.935(35) (1)0.799(35) Avg from Scherrer Analysis Integral BreadthFWHM

86
Center for Materials Science and Engineering Manually Inserting Peak Profiles Click on the ‘Profile Edit Cursor’ button Left click to insert a peak profile Right click to delete a peak profile Double-click on the ‘Profile Edit Cursor’ button to refine the peak

87
Center for Materials Science and Engineering Examples Read Y2O3 on ZBH Fast Scan.sav –make sure instrument profile is “IAP XPert FineOptics ZBH” –Note scatter of data –Note larger average crystallite size requiring good calibration –data took 1.5 hrs to collect over range 15 to 146° 2 –could only profile fit data up to 90° 2 ; intensities were too low after that Read Y2O3 on ZBH long scan.sav –make sure instrument profile is “IAP XPert FineOptics ZBH” –compare Scherrer and Size-Strain Plot –Note scatter of data in Size-Strain Plot –data took 14 hrs to collect over range of 15 to 130° 2 –size is 56 nm, strain is 0.39% by comparison, CeO 2 with crystallite size of 3 nm took 41min to collect data from 20 to 100° 2 for high quality analysis

88
Center for Materials Science and Engineering Examples Load CeO2/BN*.xrdml Overlay PDF card –shift in peak position because of thermal expansion make sure instrument profile is “IAP XPert FineOptics ZBH” look at patterns in 3D view Scans collected every 1min as sample annealed in situ at 500°C manually insert peak profile use batch mode to fit peak in minutes have record of crystallite size vs time

89
Center for Materials Science and Engineering Examples Size analysis of Si core in SiO2 shell –read Si_nodule.sav –make sure instrument profile is “IAP Rigaku RHS” –show how we can link peaks to specific phases –show how Si broadening is due completely to microstrain –ZnO is a NIST SRM, for which we know the crystallite size is between 201 nm we estimate 179 nm- shows error at large crystallite sizes

90
Center for Materials Science and Engineering We can empirically calculate nanocrystalline diffraction pattern using Jade 1.Load PDF reference card 2.go to Analyze > Simulate Pattern 3.In Pattern Simulation dialogue box 1.set instrumental profile curve 2.set crystallite size & lattice strain 3.check fold (convolute) with instrument profile 4.Click on ‘Clear Existing Display and Create New Pattern’ 5.or Click on ‘Overlay Simulated Pattern’ demonstrate with card observe peak overlap at 36° 2 as peak broaden

91
Whole Pattern Fitting

92
Center for Materials Science and Engineering Emperical Profile Fitting is sometimes difficult overlapping peaks a mixture of nanocrystalline phases a mixture of nanocrystalline and macrocrystalline phase

93
Center for Materials Science and Engineering Or we want to learn more information about sample quantitative phase analysis –how much of each phase is present in a mixture lattice parameter refinement –nanophase materials often have different lattice parameters from their bulk counterparts atomic occupancy refinement

94
Center for Materials Science and Engineering For Whole Pattern Fitting, Usually use Rietveld Refinement model diffraction pattern from calculations –With an appropriate crystal structure we can precisely calculate peak positions and intensities this is much better than empirically fitting peaks, especially when they are highly overlapping –We also model and compensate for experimental errors such as specimen displacement and zero offset –model peak shape and width using empirical functions we can correlate these functions to crystallite size and strain we then refine the model until the calculated pattern matches the experimentally observed pattern for crystallite size and microstrain analysis, we still need an internal or external standard

95
Center for Materials Science and Engineering Peak Width Analysis in Rietveld Refinement HighScore Plus can use pseudo-Voigt, Pearson VII, or Voigt profile functions For pseudo-Voigt and Pearson VII functions –Peak shape is modeled using the pseudo-Voigt or Pearson VII functions –The FWHM term, H K, is a component of both functions The FWHM is correlated to crystallite size and microstrain –The FWHM is modeled using the Cagliotti Equation U is the parameter most strongly associated with strain broadening crystallite size can be calculated from U and W U can be separated into (hkl) dependent components for anisotropic broadening

96
Center for Materials Science and Engineering Using pseudo-Voigt and Pears VIII functions in HighScore Plus Refine the size-strain standard to determine U, V, and W for the instrumental profile –also refine profile function shape parameters, asymmetry parameters, etc Refine the nanocrystalline specimen data –Import or enter the U, V, and W standard parameters –In the settings for the nanocrystalline phase, you can specify the type of size and strain analysis you would like to execute –During refinement, U, V, and W will be constrained as necessary for the analysis Size and Strain: Refine U and W Strain Only: Refine U Size Only: Refine U and W, U=W

97
Center for Materials Science and Engineering Example Open ZnO Start.hpf Show crystal structure parameters –note that this is hexagonal polymorph Calculate Starting Structure Enter U, V, and W standard –U standard= –V standard= –W standard= Set Size-Strain Analysis Option –start with Size Only –Then change to Size and Strain Refine using “Size-Strain Analysis” Automatic Refinement

98
Center for Materials Science and Engineering The Voigt profile function is applicable mostly to neutron diffraction data Using the Voigt profile function may tries to fit the Gaussian and Lorentzian components separately, and then convolutes them –correlate the Gaussian component to microstrain use a Cagliotti function to model the FWHM profile of the Gaussian component of the profile function –correlate the Lorentzian component to crystallite size use a separate function to model the FWHM profile of the Lorentzian component of the profile function This refinement mode is slower, less stable, and typically applies to neutron diffraction data only –the instrumental profile in neutron diffraction is almost purely Gaussian

99
Center for Materials Science and Engineering HighScore Plus Workshop Jan 29 and 30 (next Tues and Wed) –from 1 to 5 pm both days Space is limited: register by tomorrow (Jan 25) –preferable if you have your own laptop Must be a trained independent user of the X-Ray SEF, familiar with XRD theory, basic crystallography, and basic XRD data analysis

100
Center for Materials Science and Engineering Free Software Empirical Peak Fitting –XFit –WinFit couples with Fourya for Line Profile Fourier Analysis –Shadow couples with Breadth for Integral Breadth Analysis –PowderX –FIT succeeded by PROFILE Whole Pattern Fitting –GSAS –Fullprof –Reitan All of these are available to download from

101
Center for Materials Science and Engineering Other Ways of XRD Analysis Most alternative XRD crystallite size analyses use the Fourier transform of the diffraction pattern Variance Method –Warren Averbach analysis- Fourier transform of raw data –Convolution Profile Fitting Method- Fourier transform of Voigt profile function Whole Pattern Fitting in Fourier Space –Whole Powder Pattern Modeling- Matteo Leoni and Paolo Scardi –Directly model all of the contributions to the diffraction pattern –each peak is synthesized in reciprocal space from it Fourier transform for any broadening source, the corresponding Fourier transform can be calculated Fundamental Parameters Profile Fitting –combine with profile fitting, variance, or whole pattern fitting techniques –instead of deconvoluting empirically determined instrumental profile, use fundamental parameters to calculate instrumental and specimen profiles

102
Center for Materials Science and Engineering Complementary Analyses TEM –precise information about a small volume of sample –can discern crystallite shape as well as size PDF (Pair Distribution Function) Analysis of X-Ray Scattering Small Angle X-ray Scattering (SAXS) Raman AFM Particle Size Analysis –while particles may easily be larger than your crystallites, we know that the crystallites will never be larger than your particles

103
Center for Materials Science and Engineering Textbook References HP Klug and LE Alexander, X-Ray Diffraction Procedures for Polycrystalline and Amorphous Materials, 2 nd edition, John Wiley & Sons, –Chapter 9: Crystallite Size and Lattice Strains from Line Broadening BE Warren, X-Ray Diffraction, Addison-Wesley, 1969 –reprinted in 1990 by Dover Publications –Chapter 13: Diffraction by Imperfect Crystals DL Bish and JE Post (eds), Reviews in Mineralogy vol 20: Modern Powder Diffraction, Mineralogical Society of America, –Chapter 6: Diffraction by Small and Disordered Crystals, by RC Reynolds, Jr. –Chapter 8: Profile Fitting of Powder Diffraction Patterns, by SA Howard and KD Preston A. Guinier, X-Ray Diffraction in Crystals, Imperfect Crystals, and Amorphous Bodies, Dunod, –reprinted in 1994 by Dover Publications

104
Center for Materials Science and Engineering Articles D. Balzar, N. Audebrand, M. Daymond, A. Fitch, A. Hewat, J.I. Langford, A. Le Bail, D. Louër, O. Masson, C.N. McCowan, N.C. Popa, P.W. Stephens, B. Toby, “Size- Strain Line-Broadening Analysis of the Ceria Round-Robin Sample”, Journal of Applied Crystallography 37 (2004) S Enzo, G Fagherazzi, A Benedetti, S Polizzi, –“A Profile-Fitting Procedure for Analysis of Broadened X-ray Diffraction Peaks: I. Methodology,” J. Appl. Cryst. (1988) 21, –“A Profile-Fitting Procedure for Analysis of Broadened X-ray Diffraction Peaks. II. Application and Discussion of the Methodology” J. Appl. Cryst. (1988) 21, B Marinkovic, R de Avillez, A Saavedra, FCR Assunção, “A Comparison between the Warren-Averbach Method and Alternate Methods for X-Ray Diffraction Microstructure Analysis of Polycrystalline Specimens”, Materials Research 4 (2) 71-76, D Lou, N Audebrand, “Profile Fitting and Diffraction Line-Broadening Analysis,” Advances in X-ray Diffraction 41, A Leineweber, EJ Mittemeijer, “Anisotropic microstrain broadening due to compositional inhomogeneities and its parametrisation”, Z. Kristallogr. Suppl. 23 (2006) BR York, “New X-ray Diffraction Line Profile Function Based on Crystallite Size and Strain Distributions Determined from Mean Field Theory and Statistical Mechanics”, Advances in X-ray Diffraction 41, 1997.

105
Center for Materials Science and Engineering Instrumental Profile Derived from different mounting of LaB 6 In analysis of Y 2 O 3 on a ZBH, using the instrumental profile from thin SRM gives a size of 60 nm; using the thick SRM gives a size of 64 nm

Similar presentations

© 2016 SlidePlayer.com Inc.

All rights reserved.

Ads by Google